Effect of pressure and temperature on the structure and optical properties of two-dimensional lead iodide perovskites
Drushliak, Viktoriia; Szafrański, Marek; Chemical Communications 61 (2025) 8019–8022; doi:10.1039/D5CC01232E

data_7134440
_publ_section_title
;
 Effect of pressure and temperature on the structure and optical
 properties of two-dimensional lead iodide perovskites
;
_journal_issue                   44
_journal_name_full               'Chemical Communications'
_journal_page_first              8019
_journal_page_last               8022
_journal_paper_doi               10.1039/D5CC01232E
_journal_volume                  61
_journal_year                    2025
_chemical_formula_sum            'C H6 Cs I4 N3 Pb'
_chemical_formula_weight         907.79
_chemical_name_systematic        'Cesium guanidinium lead tetraiodide'
_space_group_crystal_system      orthorhombic
_space_group_IT_number           58
_space_group_name_Hall           '-P 2 2n'
_space_group_name_H-M_alt        'P n n m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     heavy
_audit_creation_date             2025-02-26
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_audit_update_record
;
2025-03-03 deposited with the CCDC.	2025-04-23 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   17.475(19)
_cell_length_b                   11.8768(5)
_cell_length_c                   11.5309(4)
_cell_measurement_pressure       4510000(30000)
_cell_measurement_reflns_used    2235
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.9670
_cell_measurement_theta_min      2.4440
_cell_volume                     2393(3)
_computing_cell_refinement       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/2 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS  (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.3200
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.238
_diffrn_measured_fraction_theta_max 0.192
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
  1  \f    -35.00  19.80   0.40   65.00   0.00 -30.00   0.00    --   137
  2  \f    140.00 200.00   0.40   65.00   0.00 -30.00   0.00    --   150
  3  \f    160.00 216.80   0.40   65.00   0.00  30.00   0.00    --   142
  4  \f    -20.00  34.80   0.40   65.00   0.00  30.00   0.00    --   137
  5  \w    -24.00  24.00   0.40   65.00    --   30.00  39.46 -12.90  120
  6  \w    -24.00  24.00   0.40   65.00    --   30.00  39.46 167.10  120
  7  \w    -50.00  10.00   0.40   65.00    --  -30.00  39.46 167.10  150
  8  \w    -50.00  10.00   0.40   65.00    --  -30.00  39.46 -12.90  150
  9  \w    -64.00  -8.00   0.40   65.00    --  -30.00  81.40 -28.90  140
 10  \w    -64.00  -8.00   0.40   65.00    --  -30.00  81.40 151.10  140
 11  \w    -19.00   7.80   0.40   65.00    --   30.00  81.40 151.10   67
 12  \w    -19.00   7.80   0.40   65.00    --   30.00  81.40 -28.90   67
 13  \w    -43.00 -21.00   0.40   65.00    --   30.00 134.60 -56.90   55
 14  \w    -43.00 -21.00   0.40   65.00    --   30.00 134.60 123.10   55
 15  \w    -90.00 -36.00   0.40   65.00    --  -30.00 134.60 123.10  135
 16  \w    -90.00 -36.00   0.40   65.00    --  -30.00 134.60 -56.90  135
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini ultra'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0401561000
_diffrn_orient_matrix_UB_12      -0.0033211000
_diffrn_orient_matrix_UB_13      0.0034652000
_diffrn_orient_matrix_UB_21      0.0030335000
_diffrn_orient_matrix_UB_22      0.0558833000
_diffrn_orient_matrix_UB_23      -0.0218710000
_diffrn_orient_matrix_UB_31      -0.0014385000
_diffrn_orient_matrix_UB_32      0.0213809000
_diffrn_orient_matrix_UB_33      0.0576428000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0899
_diffrn_reflns_av_unetI/netI     0.0319
_diffrn_reflns_Laue_measured_fraction_full 0.238
_diffrn_reflns_Laue_measured_fraction_max 0.192
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            9315
_diffrn_reflns_point_group_measured_fraction_full 0.238
_diffrn_reflns_point_group_measured_fraction_max 0.192
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.552
_diffrn_reflns_theta_min         2.462
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    27.369
_exptl_absorpt_correction_T_max  0.431
_exptl_absorpt_correction_T_min  0.218
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.53 (Rigaku Oxford Diffraction, 2019)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model (Absorb Angel (2004) J. Appl. Cryst. 37:486-492)
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    5.039
_exptl_crystal_description       plate
_exptl_crystal_F_000             3056
_exptl_crystal_preparation       'mounted in a diamond-anvil cell '
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.039
_refine_diff_density_min         -1.964
_refine_diff_density_rms         0.269
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     67
_refine_ls_number_reflns         613
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.056
_refine_ls_R_factor_all          0.1059
_refine_ls_R_factor_gt           0.0765
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0573P)^2^+466.9149P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1779
_refine_ls_wR_factor_ref         0.1971
_reflns_Friedel_coverage         0.000
_reflns_number_gt                406
_reflns_number_total             613
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d5cc01232e2.cif
_cod_data_source_block           CsGPbI4_4_52
_cod_depositor_comments
'Adding full bibliography for 7134427--7134444.cif.'
_cod_database_code               7134440
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_max   0.407
_shelx_estimated_absorpt_t_min   0.084
_exptl_absorpt_special_details
;
Data were collected at room temperature and pressure of 4.51(3) GPa
(4510000 kPa). 
Pressure was determined by monitoring the shift of the ruby
R1-fluorescence line.
"_diffrn_measured_fraction_theta_full" value is low, because 
the access to the reciprocal space is restricted due to the use of
the diamond anvil cell.
;
_exptl_oxdiff_absorpt_process_details
;
Gaussian integration over a grid
of 16 x 16 x 16 points =  4096 total grid points
  Based upon method of Burnham (1966)

 Data corrected for diamond-anvil cell absorption
 Note that exptl_absorpt_correction_tmin and _tmax
 the total correction factors applied to the intensities
 The individual factors are: 
         range of dac transmission factors (min-max)      0.694     0.726
         range of gasket transmission (min-max)           0.566     1.000
         range of P media transmission (min-max)          1.000     1.000

 thickness of diamond anvil 1:  8.000 mm, mu =  0.0200 mm-1
       thickness of platten 1:  0.000 mm, mu =  0.0000 mm-1

 thickness of diamond anvil 2:  8.000 mm, mu =  0.0200 mm-1
       thickness of platten 2:  0.000 mm, mu =  0.0000 mm-1

    Gasket shadowing corrections were made based upon
    Gasket thickness = 300.0 microns, radius = 174.0 microns
    Gasket absorption coeff =        30.30 mm-1
    REFLECTION WAS CONSIDERED TOTALLY OBSCURED IF 
 FRACTION CRYSTAL ILLUMINATED WAS LESS THAN 0.00

    Non-absorbing pressure medium
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All N(H,H) groups
2. Restrained distances
 C1-N12
 1.3 with sigma of 0.02
 C2-N21
 1.3 with sigma of 0.02
 C2-N22
 1.3 with sigma of 0.02
 C1-N11
 1.3 with sigma of 0.02
3. Others
 Fixed Sof: H12A(0.5) H12B(0.5) H22A(0.5) H22B(0.5)
4.a X=CH2 refined with riding coordinates:
 N11(H11A,H11B), N12(H12A,H12B), N21(H21A,H21B), N22(H22A,H22B)
;
_shelx_res_checksum              26503
_shelx_hkl_checksum              66158
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.519
_oxdiff_exptl_absorpt_empirical_full_min 0.596